Research Article Design of Polymeric Nanofiber Research Article Design of Polymeric Nanofiber Gauze
Embed Size (px)
Transcript of Research Article Design of Polymeric Nanofiber Research Article Design of Polymeric Nanofiber Gauze
Research Article Design of Polymeric Nanofiber Gauze Mask to Prevent Inhaling PM2.5 Particles from Haze Pollution
Xingzhou Li1 and Yan Gong2
1Beijing No. 35 High School, Beijing 100032, China 2Department of Materials Science and Engineering, Beijing Institute of Fashion Technology, Beijing 100029, China
Correspondence should be addressed to Yan Gong; firstname.lastname@example.org
Received 23 February 2015; Accepted 1 April 2015
Academic Editor: Qichen Wang
Copyright © 2015 X. Li and Y. Gong. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Recently, PM2.5 (particulate matter with diameter of 2.5 micron or less) has become a major health hazard from the polluted air in many cities in China. The regular gauze masks are used to prevent inhaling the PM2.5 fine particles; however, those masks are not able to filter out the PM2.5 because of the large porosity of the mask materials. Some well-prevented masks usually have poor breathability, which increases other health risks. In this study, a polysulfone based nanofiber for mask filtration material was synthesized by electrospinning.That nanofiber mask material was characterized by SEM, air permeability test, and PM2.5 trapping experiment. The results indicate that nanofiber mask material can efficiently filter out the PM2.5 particles and simultaneously preserve a good breathability. We attribute such improvement to the nanoscaled fibers, having the same porosity as that of regular gauze mask but with extremely reduced local interfiber space.
PM2.5 (particulatematterwith diameter of 2.5micron or less) in polluted air can directly go through the lung alveolar to cause many diseases including asthma . Recently, many Chinese cities are covered by haze air. Figure 1 showed the polluted air in Beijing. The heavy metals adhered on PM2.5 particles may even lead to severe chronic health problems such as cancer after long-term exposure under the particles contained environment .
In order to prevent inhaling PM2.5 in haze, people wear regular gauze masks. Most of those masks are made of non-woven fabric, activated carbon, or cotton which has fiber diameter of several micrometers . They have significant shortcoming of poor PM2.5 rejection and low air permeability .
In this paper, a novel polymeric nanofiber masks were synthesized by electrospinning. Such masks based on nanofibers are expected to well prevent the PM2.5 particles and maintain a good air permeability. These nanofibers can be potentially developed to high efficiency and low cost mask product.
2. Materials and Methods
2.1. Experiment Materials. Polysulfone, acetone, polyethy- lene oxide, and dimethyl acetamidewere purchased fromBei- jing Chemical Factory, China. Medical clinic masks, medical operating room masks, ITO PM2.5 masks, N95 respirator, and R95 masks were purchased from Tianjin Youkang med- ical and health care products factory. All chemicals were of analytical grade and were used without further purification.
2.2. Procedure for Electrospinning. Polysulfone solution was prepared at a concentration of 18 wt% by dissolving in DMAc/acetone (9 : 1) with vigorous stirring. The prepared solution was kept overnight without stirring under room temperature to remove air bubbles. For the electrospinning, the 18 wt% polysulfone solutions were filled into a syringe with a metal needle connected with a high-voltage power supply (Tianjin Dongwen High Voltage Co., China). The voltage is 13 KV and the distance between the needle and the aluminium foil is 13 cm. The polymer solution was fed at a constant rate of 0.4mL/h by using a syringe pump.
Hindawi Publishing Corporation Journal of Chemistry Volume 2015, Article ID 460392, 5 pages http://dx.doi.org/10.1155/2015/460392
2 Journal of Chemistry
Table 1: Electrospinning conditions.
Polymer Solvent Humidity Flow rate Voltage Distance Time
Polysulfone 1.8 g/polyethylene oxide 0.018 g
Dimethylacetamide 9mL/acetone 1mL 53% 0.4mL/h 13 kV 13 cm
15min 30min 60min
Figure 1: Typical haze in Beijing.
The nanofibers were collected on the surface of a non-woven PP on the grounded aluminium foil. The collective time of nanofibers was 15, 30, and 60min.More detailed information was shown in Table 1.
2.3. Morphology Observation. The membranes were dried in vacuo and sputtered gold before observation. The mor- phology of nanofiber membranes was imaged by scanning electron microscopy (SEM, Hitachi T-1000, Japan).
2.4. Permeability Simulation Test. Permeability simulation test device mainly includes a pump, a pressure differential gauge, a meter, and bronchus. The nanofiber matts and the commercial masks as control group were clamped by a well- sealed testing chamber, which was connected with a syringe at top, install a pressuremeter at the side exit.The bottom side of the chamber was open to the ambient air. Counterweights were placed on the syringe to adjust the pressure inside the testing chamber. The resulting pressure above the nanofiber matts was measured by the pressure meter.
2.5. Intercept Rate Test. Intercept experimental equipment was conducted in a nuclear particle counter (Model of CPC 3772 made in TSI Company). That counter can measure the concentration of particles (diameter between 10 and 2500 nm) in the air. The particle concentration in air repre- sented the PM2.5 intercept rate of the filtration material.
2.6. Data Analysis. All data were means ± SD from three independent experiments. Comparisons between multiple groups were performed with the ANOVA test by SPSS. 𝑃 values less than 0.05 were considered statistically significant.
15min 30min 60min
Figure 2: Nanomasks on non-woven fabrics.
3.1. Morphology Observation. Figure 2 is the picture of nanofibers on the non-woven fabric. All the masks are white in color and homogeneously distributed on the non-woven fabric. The thickness of the electrospun fiber matts was at the rank of 15min < 30min < 60min.
According to the SEM images, the nanofibers of 15min electrospinning were about 500–800𝜇m in diameter with random orientation and high porosity (Figure 2). The interdistance among the nanofibers is about 1–3 𝜇m. The nanofibers with 30 and 60min electrospinning showed sim- ilar morphology to those of 15min except for their higher thickness (data not shown).
3.2. Permeability Test. The permeability of the nanofiber masks was then compared with the commercial masks of disposable non-woven face mask, non-woven mask for oper- ation room, Ito PM2.5, N95, and R95 (Figure 4). As listed in Table 2, the pressure drop of three nanofiber masks was 15min < 30min < 60min. Compared with the commercial masks, the disposable non-woven face mask showed the lowest pressure drop, while the R95 had the highest barrier to air permeability.The low pressure drop indicated the good permeability.
3.3. Intercept Rate Test of PM2.5 by Nanofiber Masks. Table 3 showed the PM2.5 rejection capability of each mask in the intercept rate test. The rejecting ratio was calculated by the rejected particles/total particles in air. All the three nanofiber masks performed a high rejected effect of >90%, at the rank of 60min > 30min > 15min. For the commercial available masks, the disposable non-woven face mask showed the poorest effect on PM2.5 rejection of 32.9%, which could not match the requirement of daily use. By contrast, the R95 mask for medical use in preventing virus permeability had
Journal of Chemistry 3
Table 2: The pressure drop statistics in permeability test.
Masks Import (KP) Export (KP) Pressure drop (KPa) Disposable non-woven face mask 1.23 1.52 Δ0.29 Non-woven mask for operation room 1.05 1.695 Δ0.645 Ito PM2.5 1.045 1.7 Δ0.655 N95 1.125 1.635 Δ0.51 R95 1.06 1.685 Δ0.625 Nanomask (15 minutes) 1.43 1.84 Δ0.41 Nanomask (30 minutes) 1.19 2.06 Δ0.87 Nanomask (60 minutes) 0.915 2.023 Δ1.108
Table 3: PM2.5 rejection by selected masks.
Sample Average particlenumber Rejection ratio
Indoor air (negative control) 14452.9 ± 320.6 —
Disposable non-woven face mask 9695.3 ± 57.0 32.9%
Non-woven mask for operation room 499.2 ± 7.8 96.5%
ITO PM2.5 2480.3 ± 31.1 82.8% N95 739.0 ± 11.6 94.9% R95 12.4 ± 1.2 99.9% Nanomask (15 minutes) 1318.8 ± 23.6 90.9%
Nanomask (30 minutes) 476.7 ± 8.5 96.7%
Nanomask (60 minutes) 82.2 ± 3.5 99.4%
Cellulose microfiltration membrane (positive control)
0.3 ± 0.1 100.0%
an extremely high rejection of 99.9%, which is the highest one among the selected masks in our study.
In this study, a novel nanofiber mask was synthesized by electrospinning for preventing the PM2.5 from haze air. That nanofiber mask showed better performance than the com- mercial masks in both air permeability and PM2.5 rejection.
To make a clear comparison, the advantages and dis- advantages of commercial masks have been summarized in Table 4. Most of these masks were made of non-woven fabric microfibers with large diameters of several micrometers . The thin microfiber mask such as the disposable non-woven mask, though showed excellent air permeability, performed poor rejection on PM2.5 due to the insufficient thickness
of fibers and larger interfiber space. In contrast, the thick microfiber masks of Ito PM2.5 and N95 improved the reject- ing ratio of PM2.5 to >80% which is enough for daily use. But they both had high resistance on air permeability